Controlled Trapping and Release of Quantum
Dots in a DNA-Switchable Hydrogel**
Tim Liedl, Hendrik Dietz, Bernard Yurke, and
DNA-switchable structures have been under extensive investigation
in DNA nanotechnology,  where DNA-based
supramolecular assemblies are switched between mechanically
distinct conformational states through hybridization
with DNA “fuel” strands. Reversibility is achieved by displacing
previously added fuel strands from the assembly in
a branch-migration process.  This operation principle has
been recently applied to realize a switchable polyacrylamide
(PAAm) hydrogel with controllable macroscopic rheological
properties.  In the present study, we investigate the nanoscopic
aspects of this system in detail using fluorescent semiconductor
quantum dots (QDs) as probe particles. The diffusion
properties of the QDs in the gel are studied using
single-molecule fluorescence microscopy and fluorescence
correlation spectroscopy. Trapping and DNA-triggered release
of the nanoparticles is directly visualized, demonstrating
the potential of the DNA-switchable gel as a controlled
release system with possible applications in drug delivery.
PAAm gels are usually synthesized by mixing acrylamide
monomers, crosslinkers, and water in a certain ratio, followed
by initiation of polymerization with a catalyst. The resulting
polyacrylamide chains are chemically inert and biocompatible.
 Numerous crosslinking agents can be used to
tune the properties of PAAm gels.  Using double-stranded
DNA as a reversible crosslinker provides a number of advantages:
the resulting gel is biocompatible and sequence
programmable; the mechanical properties and the pore size
of the crosslinked gel can be adjusted by the length of the
[*] Dr. T. Liedl, Dr. F. C. Simmel
Department of Physics and Center for Nanoscience
Geschwister-Scholl-Platz 1, 80539 München (Germany)
Dr. H. Dietz
Physik Department E22 and Center for Nanoscience TU München
James-Franck-Straße, 85748 Garching(Germany)
Dr. B. Yurke
Bell Laboratories, Alcatel-Lucent
600 Mountain Ave, Murray Hill, NJ 07974 (USA)
[**] We thank R. Sperlingand W. J. Parak for supplyingus with quantum
dots, T. Schubert for trackingsoftware, and J. O. Rädler, N.
A. Langrana, R. A. Neher, and M. Rief for helpful discussions.
This work was funded by the IDK-NBT, the DFG (Emmy Noether
Grant to FCS and Nanosystems Initiative Munich), and the Bavarian
StMWFK (Neue Werkstoffe).
Supportinginformation for this article is available on the WWW
under http://www.small-journal.com or from the author.
DNA crosslinker strands, and the melting temperature of
the gel can be controlled by the sequence and length of the
For the synthesis of the DNA-switchable gel, two noncomplementary
Acrydite-modified oligonucleotides,  A
and B, are separately copolymerized with acrylamide (4%
w/v) and thereby incorporated into the PAAm chains.
Mixing of the two solutions yields a highly viscous fluid,
which, in our experiments, is complemented with fluorescent
colloidal semiconductor quantum dots as tracer particles.
Fluorescent QDs are easy to track with single-molecule
fluorescence techniques and they are available with a wide
variety of functionalizations for biomedical applications. 
Addition of gelation oligonucleotides complementary to
the Acrydite strands transforms the fluid PAAm/nanoparticle
mixture into a solid gel (Figure 1), trapping the particles.
The DNA crosslinker strands are equipped with an additional,
unhybridized “toehold” section that acts as a “recognition
tag” for DNA release strands.  When release strands
fully complementary to the crosslinker strands are added to
the gel, they attach to the toeholds and remove the crosslinker
strands via branch migration. The gel dissolves into a
solution, liberating the trapped particles. For a 4% acryl-
ACHTUNGTRENUNGamide “one-dimensional” (1D) gel, that is, for unlinked
linear polymer strands, a typical pore size much larger than
the particle diameter is expected, which is considerably reduced
by the crosslinking process. The crosslinking density
used in our experiments corresponds to a value of %C=
0.16 in a conventional PAAm gel crosslinked with N,N’methylene
bisACHTUNGTRENUNG(acrylamide). Compared to typical polyacrylamide
gels used for gel electrophoresis, the DNA–PAAm
gel is sparsely crosslinked. For a bis-crosslinked PAAm gel
with the same parameters, a pore size of r p>100 nm would
be expected.  Nevertheless, we experimentally observe that
the DNA-switchable gel is capable of controllably trapping
and releasing nanoparticles with a diameter on the order of
To characterize the trapping and release process in
detail, the diffusion behavior of our tracer particles was
studied in the sol and gel states of the switchable gel. As
tracer particles, we used CdSe/ZnS QDs (l em=565 nm) with
a “bare” radius of roughly 6 nm. The QDs were made water
soluble by a polymer coating  that slightly increased their
radius. As described previously,  the radius of the coated
QDs was determined using fluorescence correlation spectroscopy
(FCS). FCS measurements on free QDs in water
yielded a diffusion constant of D H2O =29 0.5 mm 2 s 1 (Figure
2b). Using the Stokes–Einstein (SE) equation this value
can be translated into a hydrodynamic radius of the particles
of 7.4 0.6 nm. We then determined the diffusion properties
of the QDs for the two states of the gel using both
single-molecule fluorescence microscopy and FCS. [10,11] In
the unlinked hydrogel matrix the diffusion constant dropped
to D FCS,unlinked =6.6 0.3 mm 2 s 1 (Figure 2b). Again using the
SE equation, one can estimate the (local  ) viscosity of the
unlinked gel matrix to be h=4.8 0.5 mPas. Tracking individual
QDs in the unlinked gel matrix by fluorescence microscopy
(Figure 2c,d) yields a diffusion constant of
D Tracking,unlinked =6.3 0.4 mm 2 s 1 , which agrees well with the
1688 2007 Wiley-VCH VerlagGmbH & Co. KGaA, Weinheim small 2007, 3, No. 10, 1688 – 1693
Figure 1. Operation principle of the DNA-switchable gel used for nanoparticle delivery. Water-soluble,
polyACHTUNGTRENUNGmer-coated nanocrystals trapped reversibly in a DNA-crosslinked polyacrylamide hydrogel (left) can
be liberated by unlinking the gel with DNA “release” strands. As a result, the particles can leave the
unlinked gel (right), and a DNA waste duplex composed of the crosslinking and the release strand is
formed. The unlinked gel can be reorganized by adding the crosslinking strand again.
Figure 2. Time trace of QDs in the unlinked gel mixture. The time traces were obtained by stacking
3000 images (128”128 pixel 2 =28”28 mm 2 , recorded at 35.7 Hz) with a distance of 0.28 pixel and subsequent
tilting of the stack by 908 around its x- ory-axis. The abscissa then corresponds to 100 ms per
pixel from left to right, while the ordinate displays the projection of the former x- ory-axis. b) Autocorrelation
functions obtained from FCS measurements of quantum dots in water and in the unlinked gel
matrix fitted with Equation (1). The diffusion constant in water is D H2O =29 0.5 mm 2 s 1 and
D FCS,unlinked =6.6 0.3 mm 2 s 1 in the unlinked gel solution. &: water; *: unlinked solution. Red line: Fit
(b=1); green line: Fit (b=0.9). Already for the unlinked matrix the fit yields a value of b
Figure 3. a) Five sections of time traces recorded during the crosslinking process. Each section is approximately
8 s long and was taken 5, 10, 20, 60, and 120 min after the addition of the crosslinking DNA
strand. With ongoing crosslinking, more and more particles get trapped. b) Five sections of time traces
recorded during the release process. Each section is around 8 s long and was taken 0, 5, 15, 25, and
60 min after the addition of the release DNA strand. With time the particles are uncaged, although the
freedom of the unlinked matrix is not completely recovered. c) 1500 images of the crosslinked gel
recorded at 35.7 Hz of a z-scan at 500 nms 1 were stacked and tilted. Almost all QDs are fixed in the
gel. d) On single bright spots, the well-known blinking behavior of QDs can be observed, which indicates
the trapping of single nanoparticles. e) Gaussian fitting the fluorescence intensities of the trapped QDs
along the y-axis allows for the accurate determination of their position with a lateral precision
Figure 4. a) Diffusion constants of the QDs during the crosslinking
and release process measured by FCS and fitted with Equation (1).
Error bars represent the standard deviation obtained from 5–10
single measurements. Inset: b-values obtained from fits with Equation
(1), indicating an increasing contribution of anomalous diffusion
for increasing crosslinking density. &: water; *: gel. b) Diffusion
constants of the QDs during the crosslinking and release process
determined from the time traces recorded by video microscopy (see
Figures 2 and 3). &: time trace; *: tracking; J: trapped particles.
c) A crosslinked gel with captured fluorescent nanoparticles disintegrates
upon addition of the release DNA and dispenses the particles
into the buffer solution. The increasing fluorescence was monitored
with a fluorescence spectrometer in constant-wavelength mode.
or antigens.  Our work demonstrates that a DNA-crosslinked
PAAm gel could be used to release nanoparticles as
potential drug-delivery vehicles in response to the presence
of trigger DNA or RNA molecules. Whether our system—
implemented as DNA-crosslinked microgel beads—could be
used for in vivo drug delivery depends on a variety of factors.
Drug release could be triggered by extracellular DNA
or RNA, which is occasionally observed in cancer patients.
 Response to intracellular RNA signals, however,
requires the uptake of the microgel beads by cells. In either
case, the concentration of naturally occurring nucleic acids
may be too low to trigger drug release efficiently. This could
be remedied, for instance, by implementation of a DNAbased
signal-amplification scheme.  A more realistic scenario
involves incorporation of aptamers or allosteric aptazymes.
 Aptazymes could be used to release DNA or
RNA strands in response to extracellular molecular signals.
The released nucleic acids would then trigger the release of
nanoparticles from the gel. The same strategy could be used
to trigger the release of drugs from pure DNA hydrogels 
with smaller pore sizes.
In conclusion, we have studied the diffusion properties
of fluorescent semiconductor nanoparticles in a DNAswitchable
hydrogel using single-QD tracking and fluorescence
correlation spectroscopy. We have demonstrated that
DNA-crosslinked hydrogels are capable of trapping and releasing
nanoparticles on demand. Nanoparticles are trapped
during the crosslinking process even though their diameter
is smaller than the mean pore size. Our system, or a modification
thereof, may find application as a switchable material
for the controlled release of nanoscale agents.
Sample preparation: CdSe/ZnS nanocrystals (Quantum Dot
Corporation (Invitrogen), Berkeley, CA; emission maximum
565 nm) were capped with a polymer coating as described
before.  Acrydite-modified DNA (A: 5’-Acrydite-CGG CCT GAA
GCC TCC GTG TG-3’, B:5’-Acrydite-AAG CAC TCT TCT CCT CTC TG
3’) was purchased from IDT (Coralville, IA), linker strand (L: 5’-
ATC GCA CGC CCA GAG AGG AGA AGA GTG CTT CAC ACG GAG GCT
TCA GGC CG-3’) and release strand (R: 5’-CGG CCT GAA GCC TCC
GTG TGA AGC ACT CTT CTC CTC TCT GGG CGT GCG AT-3’) from biomers.net,
Ulm, Germany. Stock solutions of strand A and B were
prepared separately at 3 mm DNA concentration. The stock solution
contained: 10 mm Tris, 1 mm ethylene diamine tetraactetic
acid (EDTA; pH 8.0) buffer, 200 mm NaCl, 4% acrylamide, 3 mm
DNA strand A or B and deionized water. Directly after mixing, nitrogen
was bubbled through this solution for 5 min. Initiator mixture
((NH 4) 2S 2O 8 (0.05 g) and N,N,N’,N’-tetramethylethylenediamine
(TEMED; 25 mL, Sigma, Germany) in H 2O (0.5 mL)) was
added to a final concentration of 1.4 % followed by bubbling nitrogen
for an additional 5 min. The stock solutions were mixed
1:1 and 20 mL droplets containing 10 nm QDs were placed in
coverslip chambers (Nunc, Wiesbaden, Germany) for FCS measurements.
For video microsACHTUNGTRENUNGcopy, the gel containing 100 pm QDs
and was placed into a silicon grease ring of 5-mm diameter on
a glass coverslip. To crosslink the polyacrylamide solution, linker
small 2007, 3, No. 10, 1688 – 1693 2007 Wiley-VCH VerlagGmbH & Co. KGaA, Weinheim www.small-journal.com 1691
strands L were added to a final concentration of 0.5 mm, corresponding
to a crosslink density of 33%. Dissolution of the gel
was achieved by adding a twofold excess of release strand R.
FCS Measurements: FCS measurements were performed on a
commercial FCS setup (microscope Axiovert 200 with 40”C-
Apochromat water immersion objective (NA 1.2) and ConfoCor2
module, Carl Zeiss, Jena, Germany). For excitation, the 488-nm
line of an argon-ion laser was used. Only 1% of the maximum illumination
intensity of 2.91 mW was used to minimize saturation
effects.  The emitted light was sent through a 50/50
beamsplitter and fed into two identical independent detection
channels with 505-nm long-pass filters and pinholes of 70-mm
diameter. The signals of the avalanche photodiode detectors
were cross correlated to remove artifacts such as detector afterpulsing.
A detailed description of FCS theory and techniques has
been published before.  FCS measurements of fluorescent
nanocrystals [10,27] differ from those on organic fluorophores, as
QDs exhibit no triplet behavior but show blinking on all timescales
from nanoseconds to seconds. The distribution of blinking
times follows a power law.  As for organic fluorophores, the
fluorescence decay time of QDs of a few nanoseconds is too fast
to be detected in an FCS measurement. Since, until now, no analytical
expression to fit FCS data obtained from fluorophores exhibiting
power-law-dependent blinking behavior could be derived,
we fitted the curves with a simple FCS model that only
takes diffusion into account. For calibration of the sample
volume (i.e., to determine the parameters r 0 and z 0, the radius
and the longitudinal extension of the focal volume, respectively)
the dye Alexa 488 (D=316 mm 2 s 1 , Molecular Probes) was
used. The triplet behavior of Alexa 488 was taken into account
during calibration. For all measurements r 0 was found to be between
180 and 190 nm. The ratio z 0/r 0 was always between 6
and 7. The autocorrelation functions obtained from QD measurements
were fitted with an expression for freely diffusing particles
without the term describing the triplet behavior: [16,26]
GðtÞ ¼ 1
1 þ t
1 þ r2 0
The two free parameters are the mean number of particles N
in the focal volume and the diffusion time t D. To test the data for
signatures of anomalous diffusion, the exponent b was introduced
as a third free parameter. Each FCS data point was generated
from at least 5”30 s measurement times.
Single-molecule fluorescence microscopy: We used a homebuilt
single-molecule, objective-type TIR fluorescence microscope
in epifluorescence mode to image single fluorescent quantum
dots. Core elements are a sensitive EM-CCD Camera (Andor iXON
Du-879) and a high numerical aperture objective (Carl Zeiss,
Alpha Plan Fluar, 100 ”NA 1.45). For excitation we used continuous
wave (cw) laser light at 473 nm with a sample plane intensity
of approximately 10 kWcm 2 . Fluorescence emission was collected
at 508 10 nm. Kinetic image series were collected with
25 ms exposure time and treated with Image J software in order
to calculate collapsed fluorescence image time traces.
Fluorescence spectroscopy: Approximately 5 mL of the crosslinked
gel, loaded with 20 nm QDs, were placed on the bottom
of a glass cuvette containing 300 mL TE buffer (200 mm NaCl).
The cuvette was mounted in a fluorescence spectrometer (Jobin
Yvon Fluorolog-322). In order to collect fluorescence only from
released particles, the excitation light (480 nm) was precluded
from the gel itself. Fluorescence was collected at 525 nm. After
30 min 10 mL of release DNA (3 mm) were added. To overcome
slow diffusion of the particles in the comparably large cuvette
volume, the cuvette was shaken gently between the measurements.
Videos of gel-triggered gel dissolution are available in
the Supporting Information.
diffusion · DNA structures · fluorescence · nanoparticles ·
 a) N. C. Seeman, Nature 2003, 421, 427; b) F. C. Simmel, W. U.
Dittmer, Small 2005, 1, 284; c) J. Bath, A. J. Turberfield, Nat.
Nanotechnol. 2007, 2, 275.
 B. Yurke, A. J. Turberfield, A. P. Mills, F. C. Simmel, J. L. Neumann,
Nature 2000, 406, 605.
 D. C. Lin, B. Yurke, N. A. Langrana, J. Biomech. Eng. 2004, 126,
 a) W. D. Novaes, A. Berg, Aesthetic Plast. Surg. 2003, 27, 376;
b) V. Breiting, A. Aasted, A. Jorgensen, P. Opitz, A. Rosetzsky,
Aesthetic Plast. Surg. 2004, 28, 45; c) E. A. Smith, F. W. Oehme,
Rev. Environ. Health 1991, 9, 215.
 C. Gelfi, P. G. Righetti, Electrophoresis 1981, 2, 213.
 M. Kenney, S. Ray, T. C. Boles, BioTechniques 1998, 25, 516.
 T. Pellegrino, S. Kudera, T. Liedl, A. M. Javier, L. Manna, W. J.
Parak, Small 2005, 1, 48.
 D. L. Holmes, N. C. Stellwagen, Electrophoresis 1991, 12, 612.
 T. Pellegrino, L. Manna, S. Kudera, T. Liedl, D. Koktysh, A. L.
Rogach, S. Keller, J. Radler, G. Natile, W. J. Parak, Nano Lett.
2004, 4, 703.
 T. Liedl, S. Keller, F. C. Simmel, J. O. Radler, W. J. Parak, Small
2005, 1, 997.
 D. Magde, E. L. Elson, W. W. Webb, Biopolymers 1974, 13, 29.
 X. Ye, P. Tong, L. J. Fetters, Macromolecules 1998, 31, 5785.
 M. Nirmal, B. O. Dabbousi, M. G. Bawendi, J. J. Macklin, J. K.
Trautman, T. D. Harris, L. E. Brus, Nature 1996, 383, 802.
 M. Kuno, D. P. Fromm, H. F. Hamann, A. Gallagher, D. J. Nesbitt,
J. Chem. Phys. 2000, 112, 3117.
 M. J. Saxton, Biophys. J. 1996, 70, 1250.
 M. Wachsmuth, W. Waldeck, J. Langowski, J. Mol. Biol. 2000,
 A. Pluen, P. A. Netti, R. K. Jain, D. A. Berk, Biophys. J. 1999, 77,
 Y. Qiu, K. Park, Adv. Drug Delivery Rev. 2001, 53, 321.
 a) R. Pelton, Adv. Colloid Interface Sci. 2000, 85, 1; b) X. H. Xia,
Z. B. Hu, M. Marquez, J. Controlled Release 2005, 103, 21.
 T. Miyata, N. Asami, T. Uragami, Nature 1999, 399, 766.
 a) D. Sidransky, Nat. Rev. Cancer 2002, 2, 210; b) P. Anker, J.
Lyautey, C. Lederrey, M. Stroun, Clin. Chim. Acta 2001, 313,
 a) J. S. Bois, S. Venkataraman, H. M. Choi, A. J. Spakowitz, Z. G.
Wang, N. A. Pierce, Nucleic Acids Res. 2005, 33, 4090; b) G.
Seelig, B. Yurke, E. Winfree, J. Am. Chem. Soc. 2006, 128,
 S. Seetharaman, M. Zivarts, N. Sudarsan, R. R. Breaker, Nat. Biotechnol.
2001, 19, 336.
 S. H. Um, J. B. Lee, N. Park, S. Y. Kwon, C. C. Umbach, D. Luo,
Nat. Mater. 2006, 5, 797.
1692 www.small-journal.com 2007 Wiley-VCH VerlagGmbH & Co. KGaA, Weinheim small 2007, 3, No. 10, 1688 – 1693
 a) J. Enderlein, I. Gregor, D. Patra, J. Fitter, Curr. Pharm. Biotechnol.
2004, 5, 155; b) I. Gregor, D. Patra, J. Enderlein, ChemPhys-
Chem 2005, 6, 164.
 a) P. Schwille, J. Bieschke, F. Oehlenschlager, Biophys. Chem.
1997, 66, 211; b) O. Krichevsky, G. Bonnet, Rep. Prog. Phys.
2002, 65, 251.
 a) D. R. Larson, W. R. Zipfel, R. M. Williams, S. W. Clark, M. P.
Bruchez, F. W. Wise, W. W. Webb, Science 2003, 300, 1434;
b) S. Doose, J. M. Tsay, F. Pinaud, S. Weiss, Anal. Chem. 2005,
Received: May 25, 2007
Published online on September 4, 2007
small 2007, 3, No. 10, 1688 – 1693 2007 Wiley-VCH VerlagGmbH & Co. KGaA, Weinheim www.small-journal.com 1693